Mat.No. 1.8161, DIN 58CrV4
Designation by Standards Brand Name Ravne No. Mat. No. DIN EN AISI PO186 186 1.8161 58CrV4 - - Chemical Composition (in weight %) C Si Mn Cr Mo Ni V W Others 0.59 0.28 0.90 1.05 - - 0.15 - - DescriptionAlloyed carbon steel, spring steel. ApplicationsQuenched and subsequently tempered steel for extremely wear resisting components, driving components, gears. Physical properties (avarage values) at ambient temperatureModulus of elasticity [103 x N/mm2]: 210 Densit...
Designation by Standards
|Brand Name||Ravne No.||Mat. No.||DIN||EN||AISI|
Chemical Composition (in weight %)
Alloyed carbon steel, spring steel.
Quenched and subsequently tempered steel for extremely wear resisting components, driving components, gears.
Physical properties (avarage values) at ambient temperature
Modulus of elasticity [103 x N/mm2]: 210
Density [g/cm3]: 7.85
Heat to 680-720oC, cool slowly in furnace. This will produce a maximum Brinell hardness of 248.
Temperature: 850-880oC, air.
Harden from a temperature of 820-850oC followed by oil quenching. Hardness after quenching is 60-65 HRC.
Tempering temperature: 480-650oC.
Hot forming temperature: 1050-850oC.
Forms manufactured: Please see the Dimensional Sales Program.
The information and data presented herein are typical or average values and are not a guarantee of maximum or minimum values. Applications specifically suggested for material described herein are made solely for the purpose of illustration to enable the reader to make his own evaluation and are not intended as warranties, either express or implied, of fitness for these or other puposes. There is no representation that the recipient of this literature will receive updated editions as the become available.